Corresponding author: email@example.com
Analysis of isothermal sintering of zinc-titanate doped with MgO
, S. Stevanovic1
, M. Mitric2
, M. V. Nikolic3
, M. M. Ristic4 1
Institute of Technical Sciences of SASA, Knez-Mihailova 35/IV, 11000 Belgrade,
The Vinca Institute of Nuclear Sciences, Belgrade, Serbia,
Institute for Multidisciplinary Research, Kneza Viseslava 1a, 11000 Belgrade,
Serbian Academy of Sciences and Arts, Knez-Mihailova 35/IV, 11000 Belgrade,
The aim of this work was analysis of isothermal sintering of zinc titanate ceramics doped with MgO obtained by mechanical activation. Mixtures of ZnO, TiO2 and MgO (0, 1.25
and 2.5%) were mechanically activated 15 minutes in a planetary ball mill. The powders obtained were pressed under different pressures and the results were fitted with a phenomenological compacting equation. Isothermal sintering was performed in air for 120 minutes at four different temperatures. Structural characterization of ZnO-TiO2-MgO system
after milling was performed at room temperature using XRPD measurements. DTA measurements showed different activation energies for pure and doped ZnO-TiO2 systems.
Thus addition of MgO stabilizes the crystal structure of zinc titanate.
Keywords: Pressing, Sintering, XRPD, DTA, ZnO-TiO2 system.
Historically, ZnO-TiO2 materials have been used as white color pigments and
catalysts for the desulphutization of hot coal gases [1,2]. In the last few decades, zinc-titanates have also been used as dielectric materials for microwave devices and, more preferably, for low-temperature co-fired ceramics (LTCC) [3-6].
Phase transitions in the ZnO-TiO2 system are relatively complex, and sensitive to the
start material, additives and the preparation process . Calcination of the ZnO-TiO2 system
can lead to three different phases: ZnTiO3 (hexagonal), Zn2Ti3O8 (cubic) and Zn2TiO4 (cubic)
[8-12]. Zn2TiO4 is stable from room temperature to its liquid temperature (1418 o
C), while ZnTiO3 is stable from room temperature to 945
C, which is the temperature of its separation into Zn2TiO4 and rutile-TiO2. Yamaguchi et al.  clarified that Zn2Ti3O8 is a
low-temperature form of ZnTiO3 and is stable at temperatures lower than 820 o
C. In general, these titanates are prepared by a conventional solid-state reaction, sol-gel method, etc. A number of studies up to now have been devoted to the preparation, compound formation, crystal structure, stability, additives and electrical properties of ZnTiO3 [13-16], but very few to
In this work, Zn2TiO4 ceramics with MgO addition were prepared by solid-state
reaction combined a chemical processing. MgO has been proved to be an effective sintering aid for zinc titanate ceramics [13,14]. Mechanical activation has been used to shortern the sintering procedure or lower the sintering temperature. In this case the starting powders were mechanically activated for 15 minutes because it has been demonstrated that activation of only 15 minutes very successfully promotes solid-state reaction as well as sintering processes and establishes an optimal thermal treatment of sintering at a significantly lower temperature than in case of non-activated mixture . The phase structure, pressing process as well as thermal behavior of the system were investigated.
Zn2TiO4 samples with addition of MgO = 0 - 2.50 wt.% were prepared by
conventional solid-state reaction method using ZnO (99.99% p.a. Aldrich), TiO2 (99.99% p.a.
Aldrich) and MgO (97% p.a. Merck) powders. The starting materials were mixed in ethanol in a magnetic whisk for two hours and then dried at 120oC for two hours. The powders were submitted to mechanochemical treatment for 15 minutes in a planetary ball mill device (Fritch Pulverisette 5) at the angular speed of the supporting disc set on 400 rpm. Samples were denoted according to the added oxide, ZMTO-0, ZMTO-1.25 and ZMTO-2.50. Powders were then sieved through a 0.2 mm sieve.
X-ray diffraction patterns of powder mixtures after milling were obtained using a Philips PW 1050 diffractometer with λCuKα radiation and a step/time scan mode of 0.05o/1s.
The binder-free powders were compacted using the uniaxial double action pressing process in an 8 mm diameter tool (Hydraulic press RING, P-14, VEB THURINGER). The compaction pressure was varied from 0.5 to 9 t/cm2 (49-883 MPa) to investigate the behavior of powders during compaction.
Differential thermal analysis was performed using a Shimadzu DTA-50 during non-isothermal heating from room temperature to 1100oC with a constant heating rate of 10oC/min in air atmosphere.
Compacts pressed under 4 t/cm2 pressure were placed in an alumna boat and heated in a chamber furnace (Heraeus). When the temperature of the furnace achieved 800, 900, 1000 and 1100oC, compacts were sintered isothermally in air atmosphere for 5, 15, 30, 60 and 120 minutes.
The density of specimens was calculated from precise measurements of specimen’s diameter, thickness and mass.
Results and discussion
X-ray diffraction patterns of starting activated mixtures are presented in Fig. 1. All three mixtures were submitted to the same milling conditions but yet they show some significant differences. X-ray patterns of starting mixtures containing ZnO, TiO2
-anatase together with an insignificant amount of rutile phase and a small amount of zinc-titanate phase. After 15 minutes of mechanical treatment of ZMTO-0, the intensity of ZnO diffraction peaks decreased compared to ZMTO-1.25 and ZMTO-2.50, while peaks of anatase almost completely disappeared. Intensive disappearance of an ordered crystal structure is an indicator of extremely high transfer of mechanical energy to the powder during mechanical treatment. Also, after 15 minutes of mechanical treatment detectable traces of product Zn2TiO4 were present in the ZMTO-0 mixture.
not within ZMTO-2.50 mixture.
20 30 40 50 60 70
0 20 40 60 80 100 120 140 160 180
-Zn2TiO4 -ZnO -TiO2-rutile -TiO2-anatase
2θ, (o )
Fig. 1 X-ray diffraction patterns of mechanically activated starting mixtures with different amounts of MgO
That indicates that MgO is very rigid and stable oxide and is situated around ZnO and TiO2 particles that are brittle and soft compared to MgO particles and therefore represents a
barrier for both mechanical treatment and mechanochemical reaction.
The results obtained during compaction under conditions applied are presented in Fig. 2.
0 2 4 6 8 10
0.56 0.60 0.64 0.68 0.72
Fig. 2. Ratio of green to theoretical density in dependence on the compaction pressure
In the given pressure interval, the density values decrease with MgO addition. It is important to point out that all powders show similar behavior and follow the same function during the compaction process in spite of completely different phase compositions, as we mentioned before when discussing X-ray diffraction patterns (Fig. 1.).
The specimens pressed under pressures above 4 t/cm2 were extremely fragile and thus not convenient for handling. Also, the largest variety in densities occurs until 4t/cm2 for all three mixtures, therefore that is the pressure chosen for preparing specimens for sintering process.
The results obtained during the compaction process were fitted with a phenomenological compacting equation proposed by R. Panelli and F. A. Filho :
B P A D= +
powder density at the start of compaction. Tab. I presents the values of A and B for all three mixtures. Constants A and B can be used as parameters to characterize the powder behavior during pressing. It can be stated that parameter A (inclination of the compressibility curve) provides the plastic deformation capacity of the powder in compaction.
Tab. I The value of constants characteristics of the powders
sample A B
ZMTO-0 0.1687 0.7678
ZMTO-1.25 0.1389 0.7492
ZMTO-2.50 0.1217 0.7378
Thus, as A increases, the powder undergoes increasing plastic deformation during compaction. It is also postulated that parameter B (interception of the curve resulting from Eq. (1) at zero pressure) expresses the density in the absence of pressure. Plastic materials, especially soft metals, possess the highest A values and the brittle materials-lower values, as shown in Tab. I.
In order to investigate thermal behavior of the mixtures and to calculate the activation energy of the reaction, DTA was performed during non-isothermal heating from room temperature to 1100oC with constant heating rates (10, 20 and 30oC/min) in air atmosphere. The DTA curves obtained are shown in Fig. 3. One small endo-peak is noticeable for all three mixtures in the range from 250-270oC probably due to evaporation of some impurities absorbed from the atmosphere. The two noted exothermal effects are a consequence of three processes.
The first exo-peak in the temperature range from 600 to 950oC is the result of the two exo-peaks overlapping: first one is due to arrangement of the crystal structure and crossings of ZnO and TiO2 cations between normal and inverse spinel , the second one is
due to nucleation process and spinel formation . The third exo-peak in a range from 950 to 1100oC is the result of crystal growth at higher temperatures . Considering all three peaks are near by, we can conclude that the MgO amount added in the mixtures reduce the sintering temperature slightly.
Kissinger’s  equation was used in order to determine the activation energy of zinc-titanate formation and the values for mixtures ZMTO-0, ZMTO-1.25 and ZMTO-2.50 are Ea=182.3, 224.7 and 325.1 KJmol-1, respectively. The activation energy increases with
MgO addition, indicating that higher energy is needed for reaction in the mixture with increased addition of MgO and leads us to conclude that MgO is an obstacle not only for process of mechanical activation but for zinc-titanate formation as well.
0 200 400 600 800 1000
0 50 100 150 200
ZMTO-0 ZMTO-1.25 ZMTO-2.50
Fig. 4. a), b) and c) show densities of Zn2TiO4 ceramics with MgO addition (0, 1.25
and 2.50 wt.%) sintered isothermally in air atmosphere at four different temperatures (800, 900 1000 and 1100oC). Green densities were lower with the addition of MgO and were 67.5, 64.2 and 63% of the theoretical density for ZMTO-O, ZMTO-1.25 and ZMTO-2.5 samples, respectively (theoretical densities (TD) = 5.06, 5.03 and 5.01 g/cm3 for ZMTO-0, ZMTO-1.25 and ZMTO-2.5, respectively). Densities of all three mixtures increased with sintering temperatures reading their maximum of 73% TD for the ZMTO-0 mixture, 75% TD for ZMTO-1.25 and 74.5%TD for ZMTO-2.5 mixture for 1100oC. A minimum change in density was obtained for mixtures sintered at 800 and 900oC and in spite of lowest green density in ZMTO-2.50 mixture, the maximum change in density occurs within the mentioned mixture. So, we can say that increase of MgO addition increases the densification rate, though the resulting densities are very similar.
0 20 40 60 80 100 120 67
68 69 70 71 72 73
t800 t900 t1000 t1100
sintering time, (min)
0 20 40 60 80 100 120 63
66 69 72 75
t800 t900 t1000 t1100
sintering time, (min)
0 20 40 60 80 100 120 62
64 66 68 70 72 74 76
t800 t900 t1000 t1100
sintering time, (min)
Fig. 4 Densities of Zn2TiO4 ceramics with a) 0 wt.% MgO, b) 1.25 wt.% MgO
and c) 2.50 wt.% MgO, sintered isothermally at four different temperatures
The kinetics of the sintering process of Zn2TiO4 powders with MgO addition (0, 1.25
and 2.50 wt.%) at temperatures of 1000 and 1100oC was analyzed using the phenomenological equation based on the process of transport of activated volume .
( ) ( )st st n C
where K is the process rate constant, C is a constant defining the ratio between the starting effective activated volume and the equilibrium activated volume, s is a time constant and n is a constant which depends on the process mechanism. Lower sintering temperatures were not analyzed as the shrinkage rate was very low and the process of synthesis of starting powders was still the dominant process.
20 40 60 80 100 120 0.03
0.06 0.09 0.12 0.15
ZMTO-0 ZMTO-1.25 ZMTO-2.50
sintering time, (min)
20 40 60 80 100 120
0.01 0.02 0.03 0.04 0.05 0.06
sintering time, (min)
Fig. 5. Zinc-titanate ceramics with MgO addition (0, 1.25 and 2.50 wt.%) sintered isothermally at a) 1100oC and b) 1000oC
Fig. 5. a) and b) shows that good agreement has been obtained for all powders at both sintering temperatures. The process rate constant determined for all analyzed powders was K=0.089, 0.07 and 0.146 for Zn2TiO4 with 0, 1.25 and 2.50 wt.% MgO addition sintered
at 1100oC and K=0.064, 0.054 and 0.057 for Zn2TiO4 with 0, 1.25 and 2.50 wt.% MgO
addition sintered at 1000oC. It is noticeable that this constant is lower for the lower sintering temperature. As only two sintering temperatures were analyzed it was not possible to determine the process activation energy using this parameter. The values of the constant determining the process mechanism were n=0.10, 0.14 and 0.08 for Zn2TiO4 with 0, 1.25 and
the lower sintering temperature.
The reciprocal values of this constant can be used to analyze which diffusion mechanism is dominant during the sintering process . In this case all obtained values are well above 2, confirming the dominance of the grain boundary diffusion mechanism.
The phase composition in ZnO-TiO2 with the addition of MgO = 0-2.50 wt.% solid
solutions along with the compaction process, thermal behavior and a detailed analyses of isothermal sintering was studied. The main conclusions are:
- MgO is a very rigid and stable oxide and is situated around ZnO and TiO2 particles that are
brittle and soft compared to MgO particles and therefore obstruct both mechanical treatment and the beginning of the mechanochemical reaction. Activation energies calculated from DTA measurements confirmed our statement.
- The density values of compacts decreased with MgO addition with increase in pressing pressure, although all mixtures follow the same function and can be fitted well with the Panelli and A. Filho’s compaction equation,
- Densities of all three mixtures increased with sintering temperatures reaching their maximum at 1100oC, as expected. The proposed mechanism for isothermal sintering is grain boundary diffusion.
This research is part of projects 142011 G of the Ministry for Science of the Republic of Serbia and project Φ-7 of the Fund for Scientific Research of SASA.
1. H. T. Kim, Y. Kim, M. Valant, D. Suvorov, J. Am. Ceram. Soc. 84 (2001) 1081. 2. J. H. Swisher, J. Yang, R. P. Gupta, Ind. Eng. Chem. Res. 34 (1995) 4463. 3. H. T. Kim, J. D. Byun, Y. H. Kim, Mater. Res. Bull. 33 (1998) 963. 4. H. T. Kim, J. D. Byun, Y. H. Kim, Mater. Res. Bull. 33 (1998) 975.
5. H. T. Kim, S. H. Kim, S. Nahm, J. D. Byun, Y. H. Kim, J. Am. Ceram. Soc. 82 (1999) 3043.
6. H. T. Kim, S. Nahm, J. D. Byun, Y. H. Kim, J. Am. Ceram. Soc. 82 (1999) 3476. 7. X. C. Liu, F. Gao, L. L. Zhao, C. S. Tian, J. Alloys Comp. 436 (2007) 285. 8. F. H. Dulin, D. E. Rase, J. Am. Ceram. Soc. 43 (1960) 125.
9. S. F. Bartram, R. A. Slepetys, J. Am. Ceram. Soc. 44 (1961) 493.
10. O. Yamaguchi, M. Morimi, H. Kawabata, K. Shimizu, J. Am. Ceram. Soc. 70 (1987) C97.
11. Y. S. Chang, Y. H. Chang, I. G. Chen, G. J. Chen, Y. L. Chai, J. Cryst. Growth 243 (2002) 319.
12. J. Yang, J. H. Swisher, Mater. Charact. 37 (1996) 153.
13. Y. R. Wang, S. F. Wang, Y. M. Lin, Ceram. Inter. 31 (2005) 905.
14. Y. S. Chang, Y. H. Chang, I. G. Chen, G. J. Chen, Solid St. Commun. 128 (2003) 203.
16. X. Liu et al. Mater. Res. Bull. (2007), doi:10.1016/j.materresbull.2007.03.029 17. S. K. Manik, P. Bose, S. K. Pradhan, Mater. Chem. Phys. 82 (2003) 837.
18. N. Obradovic, N. Labus, T. Sreckovic, M. M. Ristic, Mat. Sci. Forum 494 (2005) 411.
19. T. Sreckovic, N. Labus, N. Obradovic, Lj. Zivkovic, Mat. Sci. Forum, 453-454 (2004) 435.
20. V. B. Reddy, S. P. Goel, P. N. Mehrotra, Mat. Chem. Phys. 10 (1984) 365. 21. N. Nikolic, Z. Marinkovic, T. Sreckovic, J. Mat. Sci. 39 (2004) 5239. 22. H. E. Kissinger, Anal. Chem. 29 (1957) 1702.
23. M. V. Nikolic, N. Labus, M. M. Ristic, Sci. Sint. 37 (2005) 19. 24. J. L. Woolfrey, J. Am. Ceram. Soc. 55 (1972) 383.
Садржај: Циљ рада јљ била анализа изотљрмског синтљровања цинк титанатнљ
кљрамикљ допиранљ магнљзијум оксидом. Смљшљ цинк оксида, титан диоксида и
магнљзијумоксида (0, 1,25 и 2,50 тљж.%МgO) активиранљсу 15 минутаупланљтарном
млину. Прахови су затим прљсовани под различитим притисцима и рљзултати су
фитовани фљномљнолошком јљдначином прљсовања. Изотљрмско синтљровањљ јљ
извођљно у атмосфљри ваздуха 120 минута на различитим тљмпљратурама.
Структурна карактљризација систљма ZnO-TiO2-MgO послљ млљвљња извршљна јљ
рљндгљнскомдифракциономанализом. Дифљрљнцијалнатљрмалнаанализауказала јљна различитљљнљргијљ активацијљ заразличитљ концљнтрацијљдодатог адитива. Главни закључакјљдасувљћљгустинљпослљ синтљровањапостигнутљ сапраховимакојимајљ
додат магнљзијум оксид и да додатак истог стабилишљ кристалну структуру цинк
Кључне речи: Прљсовањљ, Синтљровањљ, Рљндгљнска дифракција, Дифљрљнцијална тљрмијскаанализа, Систљм ZnO-TiO2.